- Nano Express
- Open Access
Electro-Optical Properties of Low-Temperature Growth Indium-tin-oxide Nanowires Using Polystyrene Spheres as Catalyst
© Li et al. 2016
- Received: 21 December 2015
- Accepted: 27 February 2016
- Published: 9 March 2016
Polystyrene sphere was chosen as a catalyst to fabricate indium-tin-oxide (ITO) nanowires (NWs) with a low-temperature (280–300 °C) electron-beam deposition process, bearing high purity. The ITO NWs with diameter of 20–50 nm and length of ~2 um were obtained. X-ray diffraction and high-resolution transmission electron microscope show high crystal quality. The transmittance is above 90 % at a wavelength 400 nm or more, superior to the ITO bulk film. Owing to the unique morphology gradient of the ITO NWs, the effective refractive index of ITO NWs film is naturally graded from the bottom to the top. The ITO NWs have been used on LED devices (λ = 450 nm), which improved the light output power by 31 % at the current of 150 mA comparing to the one without NWs and did not deteriorate the electrical properties. Such ITO NWs open opportunity in LED devices to further improve light extraction efficiency.
- Indium-tin-oxide nanowires
- Electron-beam evaporation
- Polystyrene spheres
Indium-tin-oxide (ITO) film with high electrical conductivity and high transmittance in the visible light region is generally used in optoelectronic devices. Recently, the nanostructures of semiconducting metal oxides, such as nanorods, nanowires, and nanobelts, have attracted much attention because of their high surface-volume ratio and excellent optical/electrical properties [1–5]. Although there have been reports on the synthesis of nanostructures of ITO, most of them were grown with high-cost, low-purity, or complex processes [6–12].
In order to obtain the nanostructures with controlled size, high uniformity, and stable process, catalytic method is typically used, in which the size of the nanostructure is controlled by noble metal particles as catalyst. For example, ITO nanowires (NWs) have been grown using Au as catalyst, based on vapor-liquid-solid (VLS) method [3, 13], electron-beam deposition [14, 15], or radio frequency (RF) magnetron sputtering deposition [16,17]. However, there are some drawbacks to these methods. The VLS process needs high temperature (800~900 °C). The oblique-angle electron-beam evaporation is difficult to control cause of the shadow effect. The sputtering method is limited by the RF power and the complicated process. In addition, a common issue of these methods is the complete removal of catalyst (e.g., Au particles), impeding the fabrication of high-purity ITO NWs. Therefore, new catalysts and new processes are in need to address this issue. The polymer monodisperse microspheres with large specific surface area, strong adsorption, aggregation, and surface reaction ability have been used in the field of medical immunology, biological engineering, chemical industry, and microelectronics [18–21]. In this study, we report a method to fabricate high-quality ITO NWs, by means of electron-beam deposition with organic macromolecular material as catalyst. This method is a novel method for the preparation of ITO NWs using polystyrene (PS) as catalyst at a low temperature (280–300 °C), which has the advantages of low-cost, facile and efficient operation. This method prepares PS spheres on substrate by self-assembly, followed by the use of electron-beam evaporation to fabricate ITO NWs via PS, and then removes the PS by annealing, thereby obtained ITO NWs with better crystal quality.
In order to get more uniform distribution of PS spheres, the ICP etching is used to adjust the morphology (the scanning electron microscopy images are Appendix 1). The PS spheres without ICP etching can also serve as the catalyst to grow ITO NWs. The etching step is not necessarily to be formed. The chamber temperature was kept at 280–300 °C to ensure the surface of PS spheres remain in a molten state. For comparison, the conventional ITO films were deposited on the p-GaN surface and a quartz wafer without PS spheres in the same condition.
Without PS spheres as the catalyst, some ITO molecules are adsorbed and get together on the substrate, while another portion of the molecules is bounced back, shown in Fig. 2d. The surface adsorption capacity of substrate is relatively small, and the substrate surface is lack of induced materials. Under such conditions, the ITO material cannot grow along the fixed crystal, so the NWs cannot be fabricated. When the substrate is coated with PS spheres, the PS is in the molten state under the temperature of 300 °C, and the surface adsorption energy is larger. In this case, the ITO molecules and In-Sn alloy are adsorbed preferentially by the melted PS spheres. In-Sn alloy keeps its liquid state in PS, and then, the impinging atoms have been absorded by which, because of their higher sticking coefficient. Nucleation occurs at the droplet-PS interface, resulting in the ITO NWs growth, shown in Fig. 2e. Figure 2f is the SEM image of ITO NWs growth process in a melted PS sphere. It is seen that NWs are grown on PS sphere, and long NWs begin to intertwine with the neighboring ones. Because of the high transparency of melted PS, we can clearly see that ITO molecules are adsorbed and agglomerated in PS from the red circle area (the surface is slightly raised, and the interior is filled with granular material.), and the morphology of crystallization at the beginning stage can also be observed.
Figure 4a is the TEM image of the NWs. Figure 4b shows the high-resolution TEM (HRTEM) recorded on the marked circle regions of Fig. 4a. The HRTEM clearly shows the high degree of crystallinity with clear lattice fringes. Spacing between the lattice fringes was found to be 0.25 nm, which is well coincided with the “d” spacing of the (400) plane of the cubic phase of In2O3. Figure 4c shows the XRD line profiles for the ITO film and NWs film. The diffraction lines show the growth structure of samples. The intensity of the two major (222) and (400) peaks at 2θ = 30.5° and 35.4° in ITO NWs film is more obvious than that in ITO film. The (400)/(222) ratio in ITO NWs film is more than 100 times higher than that in ITO film (inset figure in Fig. 4c), which indicates the predominant growth direction along the  direction [7,23–25]. Using high temperature to remove the PS spheres, the strong diffraction peaks of XRD spectra and the (400)/(222) ratio have little change, indicating that the crystal quality of ITO NWs is not affected.
ITO bulk film and ITO NWs film shown in Fig. 4d were both fabricated on quartz substrate under the same condition (10 min, 0.1 nm/s) and annealed for 15 min at 470 °C under the nitrogen ambient. The transmittance of ITO NWs has improved significantly than ITO bulk film after 400 nm. The transparency of ITO NWs film at 521 nm increased to 96 % while ITO bulk film shows improvement up to 84 %. The gap between NWs is much larger than the one in dense bulk film. Although the surface with NWs has lower reflectivity but larger absorption due to light trapping effect, the transmittance still has some improvement. At the same time, we measured the sheet resistance of both by using four-probe method, the ~16 Ω/□ for ITO film and ~200 Ω/□ for ITO NWs film. The sheet resistance of ITO NWs film is larger than the bulk material, because there are some air gaps in the intertwined NWs.
The electrical and optical properties of the VLED with ITO NWs (NW-VLED) are evaluated. Figure 6b shows the current-voltage (I-V) and light output power of reference VLED (R-VLED) without ITO and NW-VLED. The operation voltages of R-VLED and NW-VLED are 4.4 and 4.7 V at 150 mA, respectively. This indicates that ITO NWs do not deteriorate the electrical properties. Moreover, the relative light output power of the NW-VLED shows about 31 % enhancement at an injection current of 150 mA comparing with that of R-VLED.As discussed previously, the enhanced output power results from the improved transmittance at the surface. The random ITO NWs could be regarded as the layers with gradient refractive index due to the arbitrary volume fractions of ITO NWs and air. Thus, more photons can escape outside the VLED structure. Therefore, ITO NWs can effectively improve the light extraction efficiency.
Figure 6c shows EL spectra of R-VLED and NW-VLED at injection currents of 150 mA. There are no significant differences in the EL peak positions (at 450 nm) of the two VLEDs with the same full width at half maximum of 22 nm. However, EL intensity obtained from the NW-VLED is larger than the R-VLED at input currents of 150 mA. These results indicate that the enhancement in EL intensity of NW-VLED is owing to the increase of light extraction efficiency by ITO NWs.
In summary, this work presents a method to grow ITO NWs at low temperature using PS spheres as catalyst. The use of PS spheres instead of metal catalyst has the advantages of low cost, easy removal, and low deposition temperature (280–300 °C). The fabricated ITO NWs have a better crystallinity, featuring the tendency to orientate vertically. The XRD reveals a cubic structure of the ITO NWs. The transmittance is above 90 % at a wavelength 400 nm or more, superior to the ITO bulk film. Owing to the unique morphology gradient of the ITO NWs, the effective refractive index is naturally graded from the bottom to the top, ideal for light extraction enhancement in LEDs. The ITO NWs have been used on LED devices (λ = 450 nm), and the light output power increased by 31 % at the current of 150 mA comparing to the one without NWs.
This work was supported by the grant from the National High Technology Research and Development Program of China (NO. 2014AA032608), the National Natural Science Foundation of China (NO. 61404101), and the China Postdoctoral Science Foundation (NO. 2014 M562415).
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
- Huh C, Kim BK, Ahn CG, Choi CJ, Kim SH (2014) Enhancement in light emission and electrical efficiencies of a silicon nanocrystal light-emitting diode by indium tin oxide nanowires. Appl Phys Lett 105:031108View ArticleGoogle Scholar
- Fung MK, Sun YC, Ng AMC, Chen XY, Wong KK, Djurisic AB, Chan WK (2011) Indium tin oxide nanowires growth by dc sputtering. Appl Phys A 104:1075–1080View ArticleGoogle Scholar
- Wang Q, Wei M, Zhi D, MacManus-Driscoll JL, Blamire MG (2006) Epitaxial growth of vertically aligned and branched single-crystalline tin-doped indium oxide nanowires arrays. Adv Mater 18:234–238View ArticleGoogle Scholar
- LaForge JM, Cocker TL, Beaudry AL, Cui K, Tucker RT, Taschuk MT, Hegmann FA, Brett MJ (2014) Conductivity control of as-grown branched indium tin oxide nanowires networks. Nanotech 25:035701View ArticleGoogle Scholar
- Deng Z, Chen M, Gu G, Wu L (2008) A facile method to fabricate ZnO hollow spheres and their photocatalytic property. J Phys Chem B 112:16–22View ArticleGoogle Scholar
- Dong H, Zhang X, Niu Z, Zhao D, Li J, Cai L, Zhou W, Xie S (2013) Indium tin oxide nanowires grown by one-step thermal evaporation-deposition process at low temperature. J Nanosci Nanotech 13:1300–1303View ArticleGoogle Scholar
- Yu HK, Lee JL (2014) Effect of ion beam assisted deposition on the growth of indium tin oxide (ITO) nanowires. Cryst Eng Comm 16:4108–4112View ArticleGoogle Scholar
- O’Dwyer C, Szachowicz M, Visimberga G, Lavayen V, Newcomb SB, Sotomayor Torres CM (2009) Bottom-up growth of fully transparent contact layers of indium tin oxide nanowires for light-emitting devices. Nature Nanotech 4:239–244View ArticleGoogle Scholar
- Wan Q, Feng P, Wang TH (2006) Vertically aligned tin-doped indium oxide nanowire arrays: epitaxial growth and electron field emission properties. Appl Phys Lett 89:123102View ArticleGoogle Scholar
- Shen Y, Turner S, Yang P, Tendeloo GV, Lebedev OI, Wu T. Epitaxy-enabled vapor-liquid-solid growth of tin-doped indium oxide nanowires with controlled orientations. Nano Lett. 14, 4342-51.Google Scholar
- Liang YC, Zhong H (2013) Self-catalytic crystal growth, formation mechanism, and optical properties of indium tin oxide nanostructures. Nanoscal Res Lett 8:358View ArticleGoogle Scholar
- Jin Y, Yi Q, Ren Y, Wang X, Ye Z (2013) Molecular mechanism of monodisperse colloidal tin-doped indium oxide nanocrystals by a hot-injection approach. Nanoscal Res Lett 8:153. http://nanoscalereslett.springeropen.com/articles/10.1186/1556-276X-8-153. doi:10.1186/1556-276X-8-153
- Fung MK, Sun YC, Ng A, Ng AMC, Djurisić AB, Chan HT, Chan WK (2011) Indium tin oxide nanorod electrodes for polymer photovoltaics. ACS Appl Mater Interfaces 3:522–527View ArticleGoogle Scholar
- Hsu MH, Yu P, Huang JH, Chang CH, Wu CW, Cheng YC, Chu CW (2011) Balanced carrier transport in organic solar cells employing embedded indium-tin-oxide nanoelectrodes. Appl Phys Lett 98:073308View ArticleGoogle Scholar
- Lin CC, Lee CT (2010) Enhanced light extraction of GaN-based light emitting diodes using nanorod arrays. Electrochem Solid-State Lett 13:H278–H280View ArticleGoogle Scholar
- Park JH, Park HK, Jeong J, Kim W, Min BK, Do YR (2011) Wafer-scale growth of ITO nanorods by radio frequency magnetron sputtering deposition. J Electrochem Soc 158:K131–K135View ArticleGoogle Scholar
- Yamamoto N, Morisawa K, Murakami J, Nakatani Y (2014) Formation of ITO nanowires using conventional magnetron sputtering. ESC Solid State Lett 3:84–86View ArticleGoogle Scholar
- Li S, Yang X, Huang W (2005) Synthesis of monodisperse polymer microspheres with mercapto groups and their application as a stabilizer for gold metallic colloid. Macromol Chem Phys 206:1967–1972View ArticleGoogle Scholar
- Cong Y, Xia T, Zou M, Li Z, Peng B, Guo D, Deng Z (2014) Mussel-inspired polydopamine coating as a versatile platform for synthesizing polystyrene/Ag nanocomposite particles with enhanced antibacterial activities. J Mater Chem B 2:3450–3461View ArticleGoogle Scholar
- Li Z, Wu C, Zhao K, Peng B, Deng Z (2015) Polydopamine-assisted synthesis of raspberry-like nanocomposite particles for superhydrophobic and superoleophilic surfaces. Colloid Surf A: Physicochem Eng Asp 470:80–91View ArticleGoogle Scholar
- Zhao K, Zhao J, Wu C, Zhang S, Deng Z, Hu X, Chen M, Peng B (2015) Fabrication of silver-decorated sulfonated polystyrene microspheres for surface-enhanced Raman scattering and antibacterial applications. RSC Adv 5:69543–69554View ArticleGoogle Scholar
- Huang Y, Yun F, Wang Y, Ding W, Li Y, Wang H, Zhang Y, Guo M, Su X, Liu S, Hou X (2014) Surface plasmon enhanced green light emitting diodes with silver nanorod arrays embedded in p-GaN. Jpn J Appl Phys 53:084001View ArticleGoogle Scholar
- Langford JI, Wilson AJC (1978) Scherrer after sixty years: a survey and some new results in the determination of crystallite size. J Appl Crystallogr 11:102–113View ArticleGoogle Scholar
- Li L, Chen S, Kim J, Xu C, Zhao Y, Ziegler KJ (2015) Controlled synthesis of tin-doped indium oxide nanowires. J Cryst Growth 413:31–36View ArticleGoogle Scholar
- Wang Y, Lu L, Wu F (2010) ITO @carbon core-shell nanowires and jagged ITO nanowires. Nanoscal Res Lett 5:1682–1685View ArticleGoogle Scholar
- Jeong H, Park DJ, Lee HS, Ko YH, Yu JS, Choi SB, Lee DS, Suh EK, Jeong MS (2014) Light-extraction enhancement of a GaN-based LED covered with ZnO nanorod arrays. Nanoscale 6:4371–4378View ArticleGoogle Scholar
- Tsai MA, Wang HW, Yu P, Kuo HC, Lin SH (2011) High extraction efficiency of GaN-based vertical-injection light-emitting diodes using distinctive indium-tin-oxide nanorod by glancing-angle deposition. Jpn J Appl Phys 50:052102View ArticleGoogle Scholar